#------------------------------------------------------------------------------
#$Date: 2022-04-15 01:40:47 +0300 (Fri, 15 Apr 2022) $
#$Revision: 274535 $
#$URL: file:///home/coder/svn-repositories/cod/cif/7/24/47/7244780.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7244780
loop_
_publ_author_name
'Wu, Wei-Wei'
'Ruan, Ze-Yu'
'Shi, Chen-Guang'
'Mai, Jin-Tao'
'Cui, Wen'
'Ni, Zhao-Ping'
'Wu, Si-Guo'
'Tong, Ming-Liang'
_publ_section_title
;
 2D/3D spin crossover porous coordination polymers based on isomeric
 tetrapyridyl benzene ligands
;
_journal_name_full               CrystEngComm
_journal_paper_doi               10.1039/D2CE00445C
_journal_year                    2022
_chemical_formula_moiety         'C28 H24 B2 Fe N6'
_chemical_formula_sum            'C39 H34 B2 Fe N6 S'
_chemical_formula_weight         696.25
_space_group_crystal_system      orthorhombic
_space_group_IT_number           65
_space_group_name_Hall           '-C 2 2'
_space_group_name_H-M_alt        'C m m m'
_atom_sites_solution_hydrogens   mixed
_atom_sites_solution_primary     dual
_audit_creation_date             2022-04-11
_audit_creation_method
;
Olex2 1.5
(compiled 2021.11.18 svn.ra9532c28 for OlexSys, GUI svn.r6429)
;
_audit_update_record
;
2022-04-13 deposited with the CCDC.	2022-04-14 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   12.0275(9)
_cell_length_b                   15.8838(11)
_cell_length_c                   9.5912(6)
_cell_measurement_reflns_used    1349
_cell_measurement_temperature    120(2)
_cell_measurement_theta_max      72.5070
_cell_measurement_theta_min      4.5940
_cell_volume                     1832.3(2)
_computing_cell_refinement       'CrysAlisPro 1.171.39.46 (Rigaku OD, 2018)'
_computing_data_collection       'CrysAlisPro 1.171.39.46 (Rigaku OD, 2018)'
_computing_data_reduction        'CrysAlisPro 1.171.39.46 (Rigaku OD, 2018)'
_computing_molecular_graphics    'Olex2 1.5 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 1.5 (Dolomanov et al., 2009)'
_computing_structure_refinement  'SHELXL 2018/3 (Sheldrick, 2015)'
_computing_structure_solution    'SHELXT 2014/5 (Sheldrick, 2014)'
_diffrn_ambient_environment      N~2~
_diffrn_ambient_temperature      120(2)
_diffrn_detector                 'CCD plate'
_diffrn_detector_area_resol_mean 5.2913
_diffrn_detector_type            AtlasS2
_diffrn_measured_fraction_theta_full 0.997
_diffrn_measured_fraction_theta_max 0.974
_diffrn_measurement_details
;
List of Runs (angles in degrees, time in seconds):

  # Type    Start    End  Width  tₑₓₚ   ω     θ     κ     φ   Frames
#--------------------------------------------------------------------------
  1  ω     -9.00  25.00   1.00    5.00    --  -41.14  38.00   0.00   34
  2  ω    -53.00 -14.00   1.00    5.00    --  -41.14  38.00   0.00   39
  3  ω     28.00  97.00   1.00    5.00    --   41.14-125.00 -30.00   69
  4  ω     75.00 100.00   1.00    5.00    --   41.14 164.00 -73.00   25
  5  ω    103.00 176.00   1.00   20.00    --  105.29  77.00 150.00   73
  6  ω     99.00 176.00   1.00   20.00    --  105.29 125.00 -90.00   77
  7  ω     23.00  51.00   1.00   20.00    --  105.29 -94.00 120.00   28
  8  ω     64.00 147.00   1.00   20.00    --  105.29 -15.00 -60.00   83
;
_diffrn_measurement_device       'four-circle diffractometer'
_diffrn_measurement_device_type  'SuperNova, Dual, Cu at home/near, AtlasS2'
_diffrn_measurement_method       'ω scans'
_diffrn_orient_matrix_type
'CrysAlisPro convention (1999,Acta A55,543-557)'
_diffrn_orient_matrix_UB_11      0.0797093000
_diffrn_orient_matrix_UB_12      0.0754947000
_diffrn_orient_matrix_UB_13      0.0115345000
_diffrn_orient_matrix_UB_21      -0.0094028000
_diffrn_orient_matrix_UB_22      0.0145714000
_diffrn_orient_matrix_UB_23      -0.1583661000
_diffrn_orient_matrix_UB_31      -0.0998157000
_diffrn_orient_matrix_UB_32      0.0591486000
_diffrn_orient_matrix_UB_33      0.0240756000
_diffrn_radiation_monochromator  mirror
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           'Cu K\a'
_diffrn_radiation_wavelength     1.54184
_diffrn_reflns_av_R_equivalents  0.0289
_diffrn_reflns_av_unetI/netI     0.0321
_diffrn_reflns_Laue_measured_fraction_full 0.997
_diffrn_reflns_Laue_measured_fraction_max 0.974
_diffrn_reflns_limit_h_max       13
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_k_max       19
_diffrn_reflns_limit_k_min       -13
_diffrn_reflns_limit_l_max       8
_diffrn_reflns_limit_l_min       -11
_diffrn_reflns_number            2274
_diffrn_reflns_point_group_measured_fraction_full 0.997
_diffrn_reflns_point_group_measured_fraction_max 0.974
_diffrn_reflns_theta_full        67.684
_diffrn_reflns_theta_max         72.856
_diffrn_reflns_theta_min         4.610
_diffrn_source                   'micro-focus sealed X-ray tube'
_diffrn_source_type              'SuperNova (Cu) X-ray Source'
_exptl_absorpt_coefficient_mu    4.106
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  0.51574
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
CrysAlisPro 1.171.39.46 (Rigaku Oxford Diffraction, 2018)
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_colour            'clear dark red'
_exptl_crystal_colour_lustre     clear
_exptl_crystal_colour_modifier   dark
_exptl_crystal_colour_primary    red
_exptl_crystal_density_diffrn    1.262
_exptl_crystal_description       block
_exptl_crystal_F_000             724
_exptl_crystal_size_max          0.271
_exptl_crystal_size_mid          0.215
_exptl_crystal_size_min          0.102
_refine_diff_density_max         0.071
_refine_diff_density_min         -0.170
_refine_diff_density_rms         0.013
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.135
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     76
_refine_ls_number_reflns         1030
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.135
_refine_ls_R_factor_all          0.0566
_refine_ls_R_factor_gt           0.0562
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.1018P)²+0.0618P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1646
_refine_ls_wR_factor_ref         0.1653
_reflns_Friedel_coverage         0.000
_reflns_number_gt                1026
_reflns_number_total             1030
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            d2ce00445c2.cif
_cod_data_source_block           4_tpbs_120K
_cod_database_code               7244780
_shelx_shelxl_version_number     2018/3
_chemical_oxdiff_usercomment     WWW
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_shelx_estimated_absorpt_t_max   0.679
_shelx_estimated_absorpt_t_min   0.402
_olex2_refinement_description
;
1. Fixed Uiso
 At 1.2 times of:
  All C(H) groups
 At 1.5 times of:
  All B(H,H,H) groups
2. Others
 Fixed Sof: C6(0.5) H6(0.5) C5(0.5) H5(0.5) C3(0.5) H3(0.5) H1A(0.25)
 H1B(0.25) H1C(0.25) C2(0.5) H2(0.5)
3.a Riding coordinates:
 B1(H1A,H1B,H1C)
3.b Aromatic/amide H refined with riding coordinates:
 C8(H8), C6(H6), C5(H5), C3(H3), C2(H2)
;
_smtbx_masks_void_probe_radius   1.2
_smtbx_masks_void_truncation_radius 1.2
_olex2_date_sample_data_collection 2021-06-24
_olex2_submission_special_instructions 'No special instructions were received'
_oxdiff_exptl_absorpt_empirical_details
;
Empirical correction (ABSPACK) includes:
- Absorption correction using spherical harmonics
- Frame scaling
;
_oxdiff_exptl_absorpt_empirical_full_max 1.797
_oxdiff_exptl_absorpt_empirical_full_min 0.772
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, z'
'-x, y, -z'
'x, -y, -z'
'x+1/2, y+1/2, z'
'-x+1/2, -y+1/2, z'
'-x+1/2, y+1/2, -z'
'x+1/2, -y+1/2, -z'
'-x, -y, -z'
'x, y, -z'
'x, -y, z'
'-x, y, z'
'-x+1/2, -y+1/2, -z'
'x+1/2, y+1/2, -z'
'x+1/2, -y+1/2, z'
'-x+1/2, y+1/2, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Fe1 Fe 1.000000 0.500000 1.000000 0.0187(11) Uani 1 8 d S T P A .
N2 N 0.8812(2) 0.500000 0.8537(3) 0.0223(13) Uani 1 2 d S T P . .
N1 N 1.000000 0.3775(3) 1.000000 0.0241(14) Uani 1 4 d S T P . .
C8 C 0.500000 0.500000 0.6419(5) 0.0264(15) Uani 1 4 d S T P . .
H8 H 0.500000 0.500000 0.740901 0.032 Uiso 1 4 calc R U P . .
C4 C 0.7033(3) 0.500000 0.6620(3) 0.0243(13) Uani 1 2 d S T P . .
C7 C 0.6026(3) 0.500000 0.5734(3) 0.0231(13) Uani 1 2 d S T P . .
C1 C 1.000000 0.3061(4) 1.000000 0.0409(18) Uani 1 4 d S T P A .
C6 C 0.7954(4) 0.4429(3) 0.8668(5) 0.0235(15) Uani 0.5 1 d . . P A -1
H6 H 0.797191 0.403859 0.941753 0.028 Uiso 0.5 1 calc R U P A -1
C5 C 0.7070(4) 0.4404(3) 0.7749(5) 0.0245(15) Uani 0.5 1 d . . P A -1
H5 H 0.649469 0.399984 0.786171 0.029 Uiso 0.5 1 calc R U P A -1
C3 C 0.7938(4) 0.5503(3) 0.6459(5) 0.0245(15) Uani 0.5 1 d . . P A -1
H3 H 0.798562 0.586378 0.567153 0.029 Uiso 0.5 1 calc R U P A -1
B1 B 1.000000 0.2044(8) 1.000000 0.131(7) Uani 1 4 d S T P . .
H1A H 0.947300 0.184255 1.067360 0.197 Uiso 0.25 1 d R U P A -1
H1B H 1.072870 0.184255 1.023560 0.197 Uiso 0.25 1 d R U P A -1
H1C H 0.979840 0.184255 0.909080 0.197 Uiso 0.25 1 d R U P A -1
C2 C 0.8786(4) 0.5495(3) 0.7424(5) 0.0228(15) Uani 0.5 1 d . . P A -1
H2 H 0.939274 0.586816 0.728268 0.027 Uiso 0.5 1 calc R U P A -1
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0181 0.0091 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
B B 0.0090 0.0039 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Fe Fe -1.1336 3.1974 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0311 0.0180 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
S S 0.3331 0.5567 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
N2 Fe1 N2 91.03(16) 9_767 10_557 ?
N2 Fe1 N2 180.0 9_767 . ?
N2 Fe1 N2 91.03(16) 2_765 . ?
N2 Fe1 N2 88.97(16) 9_767 2_765 ?
N2 Fe1 N2 180.0 10_557 2_765 ?
N2 Fe1 N2 88.97(16) 10_557 . ?
N1 Fe1 N2 90.000(1) . . ?
N1 Fe1 N2 90.000(1) . 10_557 ?
N1 Fe1 N2 90.0 . 9_767 ?
N1 Fe1 N2 90.000(1) 9_767 2_765 ?
N1 Fe1 N2 90.0 9_767 . ?
N1 Fe1 N2 90.000(1) 9_767 9_767 ?
N1 Fe1 N2 90.0 . 2_765 ?
N1 Fe1 N2 90.0 9_767 10_557 ?
N1 Fe1 N1 180.0 . 9_767 ?
C6 N2 Fe1 118.0(2) . . ?
C2 N2 Fe1 125.5(3) . . ?
C2 N2 C6 116.4(4) . . ?
C1 N1 Fe1 180.0 . . ?
C7 C8 H8 118.0 2_665 . ?
C7 C8 H8 118.0 . . ?
C7 C8 C7 124.0(4) . 2_665 ?
C5 C4 C7 117.2(3) . . ?
C3 C4 C7 126.2(3) . . ?
C3 C4 C5 116.6(4) . . ?
C8 C7 C4 117.0(3) . . ?
C8 C7 C7 118.0(2) . 10_556 ?
C7 C7 C4 125.04(18) 10_556 . ?
N1 C1 B1 180.0 . . ?
N2 C6 H6 118.8 . . ?
N2 C6 C5 122.5(4) . . ?
C5 C6 H6 118.8 . . ?
C4 C5 H5 120.5 . . ?
C6 C5 C4 119.0(4) . . ?
C6 C5 H5 120.5 . . ?
C4 C3 H3 119.6 . . ?
C4 C3 C2 120.7(4) . . ?
C2 C3 H3 119.6 . . ?
C1 B1 H1A 109.4 . . ?
C1 B1 H1B 109.4 . . ?
C1 B1 H1C 109.4 . . ?
H1A B1 H1B 109.5 . . ?
H1A B1 H1C 109.5 . . ?
H1B B1 H1C 109.5 . . ?
N2 C2 C3 124.3(4) . . ?
N2 C2 H2 117.8 . . ?
C3 C2 H2 117.8 . . ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Fe1 N2 2.002(3) 9_767 ?
Fe1 N2 2.002(3) . ?
Fe1 N2 2.002(3) 2_765 ?
Fe1 N2 2.002(3) 10_557 ?
Fe1 N1 1.946(4) 9_767 ?
Fe1 N1 1.946(4) . ?
N2 C6 1.380(5) . ?
N2 C2 1.326(5) . ?
N1 C1 1.134(8) . ?
C8 H8 0.9500 . ?
C8 C7 1.398(4) 2_665 ?
C8 C7 1.398(4) . ?
C4 C7 1.480(5) . ?
C4 C5 1.439(5) . ?
C4 C3 1.358(5) . ?
C7 C7 1.409(6) 10_556 ?
C1 B1 1.616(13) . ?
C6 H6 0.9500 . ?
C6 C5 1.382(7) . ?
C5 H5 0.9500 . ?
C3 H3 0.9500 . ?
C3 C2 1.378(7) . ?
B1 H1A 0.9598 . ?
B1 H1B 0.9599 . ?
B1 H1C 0.9599 . ?
C2 H2 0.9500 . ?
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
Fe1 N2 C6 C5 177.0(4) . . . . ?
Fe1 N2 C2 C3 -177.6(3) . . . . ?
N2 C6 C5 C4 -0.6(7) . . . . ?
C4 C3 C2 N2 1.7(7) . . . . ?
C7 C8 C7 C4 180.000(1) 2_665 . . . ?
C7 C8 C7 C7 0.000(1) 2_665 . . 10_556 ?
C7 C4 C5 C6 -174.9(4) . . . . ?
C7 C4 C3 C2 174.4(3) . . . . ?
C6 N2 C2 C3 3.8(6) . . . . ?
C5 C4 C7 C8 47.7(3) . . . . ?
C5 C4 C7 C7 -132.3(3) . . . 10_556 ?
C5 C4 C3 C2 -6.6(6) . . . . ?
C3 C4 C7 C8 -133.3(3) . . . . ?
C3 C4 C7 C7 46.7(3) . . . 10_556 ?
C3 C4 C5 C6 6.0(6) . . . . ?
C2 N2 C6 C5 -4.3(6) . . . . ?
loop_
_smtbx_masks_void_nr
_smtbx_masks_void_average_x
_smtbx_masks_void_average_y
_smtbx_masks_void_average_z
_smtbx_masks_void_volume
_smtbx_masks_void_count_electrons
_smtbx_masks_void_content
1 0.000 0.000 0.000 14.5 0.0 ?
2 -0.019 0.250 -0.752 297.4 100.1 ?
3 -0.735 0.750 -0.039 297.4 100.1 ?
4 0.500 0.500 0.000 14.5 0.0 ?
